Irradiation study of Ti-6Al-4V and Ti-6Al-4V-1B for FRIB beam dump: Experimental plan Aida Amroussia, PhD Student Chemical Engineering and Materials Science Michigan State University 1 Slide 2 Motivation Study of irradiation damage in Ti-6Al-4V and Ti-6Al-4V-1B Irradiation with different particles and energy levels: Neutron Heavy ions with low, intermediate and high energy Compare the results: Does boron addition improves mechanical properties of Ti-6Al-4V after irradiation? Are the changes in mechanical properties of the Ti-alloys similar after neutron and heavy ions irradiation? At what neutron flux ? What energy/ intensity/ dpa rate? 2 Slide 3 Ti-6Al-4V vs Ti-6Al-4V-1B AlloyTi-6Al-4VTi-6Al-4V-1B E [GPa] At RT110127 At 500 C90113 Yield Stress [MPa] At RT10001190 At 500 C450663 Ultimate Tensile Strength [MPa] At RT8271300 At 500 C430785 Minimum creep rate [s -1 ] T=500, 400 MPa1.24.10 -6 5.89.10 -8 HCF strength [MPa] At 500 C172-258314-471 3 Boron addition improves different characteristics of Ti-6Al-4V: The stability of the microstructure is increased. The specific stiffness and strengths increases to 50%. Improvement of the machinability and thermo-mechanical processing is obtained. Chen, W., C.J. Boehlert, E.A. Payzant, and J.Y. Howe. The Effect of Processing on the 455C Tensile and Fatigue Behavior of Boron-modified Ti6Al4V. International Journal of Fatigue 32, no. 3 (March 2010): 627638. Wei Chen and Carl J. Boehlert, Characterization of the Microstructure, Tensile and Creep Behavior of Powder Metallurgy Processed and Rolled Ti-6Al-4V-1B Alloy, Key Engineering Materials, 436 (2010), 195203 Slide 4 Literature review of neutron irradiation damage in Ti-6Al-4V: Yield strength saturates at irradiation doses higher than 0.3 dpa at 60 o C. No saturation at 350 o C 4 Different hardening mechanisms operate at 50 o C than at 350 o C. Tensile and fracture toughness S. Thtinen, P. Moilanen and B.N. Singh, Effect of Displacement Dose and Irradiation Temperature on Tensile and Fracture Toughness Properties of Titanium Alloys, Journal of Nuclear Materials, 367-370 (2007), 627632 Slide 5 Microstructure Temperature and dose levelMicrostructure change observations 50 o C, 0.3 dpa A high density of uniformly distributed defect clusters in the -phase No changes in the overall dislocation or phase structures 350 o C, 0.3 dpa Dislocation loops Vanadium precipitates 450 o C Dose 2.1 and 32 dpa Dislocation loops -phase precipitates in phase 550 o C 32 dpa Extensive void formation Coarse -precipitates 5 Literature review of neutron irradiation damage in Ti-6Al-4V: S. Thtinen, P. Moilanen and B.N. Singh, Effect of Displacement Dose and Irradiation Temperature on Tensile and Fracture Toughness Properties of Titanium Alloys, Journal of Nuclear Materials, 367-370 (2007), 627632 Slide 6 Irradiation and post-irradiation characterization plan: 1.Neutron irradiation 2.Heavy ion irradiation 6 Slide 7 1.Neutron irradiation Abundance of data on neutron irradiation of Ti-6Al-4V (low doses) Comparison between Ti-6Al-4V and Ti-6Al-4V-1B 7 ReferenceIrradiation FacilityReactorAtmosphereTemperatureNeutron fluenceDose  Institute of Reactor Materials, Russia IVV-2M reactorinert gas250 Cunkown 0.2 and 0.3 dpa  Ris National Laboratory, Denmark DR-3 reactor atmosphere of helium 50 C and 350 C 1.5 10^24 n/m2 (E > 1 MeV) 0.3 dpa  Atomic Energy Research Institute in Budapest VVRSZM Russian Research Reactor Cooling through He/N2 gas 150 C 1.08E20 n/cm2 (E > 1 MeV) 0.15 dpa Slide 8 1.Neutron irradiation at HFIR-ORNL Irradiation experiment: Neutron flux =1E+14n/cm 2 /sec, for E>0.183 MeV. Irradiation time: 1 cycle (23 days) Sample: 0.76 x 1.52 x 7.6 mm Temperature : 350 C Post irradiation characterization : The Materials Science and Technology Division of ORNL is equipped with remote hot cells with servo-hydraulic test systems that can perform mechanical testing: Scanning Electron Microscopy (SEM), Transmission Electron Microscopy (TEM) and Atom Probe Tomography (APT) to perform microstructural characterization. In-situ tensile testing and fracture toughness testing machines to study the mechanical properties of the neutron irradiated Ti-6Al-4V-1B. 8 Slide 9 2.Heavy ion irradiation: 9 ion energy MeV/nucleo n minimum current (Ae) flux min (ions/(cm 2.s)) required time (1UT=8 hours) Range in the material (m) Ar115 Ae 10 12 128 IRRSUD Ar 36FRIB O 18FRIB Ca 48FRIB U 238 Energy (MeV/A)1230194156 Estimated dpa/h0.32.5.10 -5 2.5.10 -4 1.5.10 -3 Total dose-0.131.358.5 Se (keV/nm)7.240.080.612.6 Table 1 Comparison between IRRSUD and FRIB beams I.Low energy irradiation at CIMAP-GANIL France Slide 10 Irradiation experiment: Samples : Dogbone samples (550-800m)and TEM samples Temperature : 350 C and RT Material: Ti-6Al-4V and Ti-6Al-4V -1B Post-irradiation characterization at MSU: In-situ tensile tests Nano-indentation TEM and SEM characterization X-Ray diffraction ( small angle diffraction) 10 I.Low energy irradiation at CIMAP-GANIL France Beam area Dogbone samples 2.Heavy ion irradiation: Slide 11 Two tests were performed at IRRSUD - CIMAP in July and October 2013 with both Ti-alloys (Ti- 6Al-4V and Ti-6Al-4V-1B) 4 irradiations ( 82 Kr at 25 and 45 MeV and 131 Xe at 92 MeV, up to 2.5 10 15 ions/cm) No evidence of phase transformation and ion track in Ti-6Al-4V promises good radiation resistance of this alloy F. Pellemoine, Nov 2013 ESAC Review - 14, Slide 11 pristine Xe 92 MeV 2 10 11 ions/cm Kr 45 MeV 5 10 13 ions/cm Ti-6Al-4V Ti-6Al-4V-1B Al-7075 Al-6061 3 glue specimen Intensity (u.a.) 2 () Preliminary results with Ti-6Al-4V Slide 12 AE total (MeV) E (MeV/u) Range (m) Se (keV/nm) I (pnA)P (W) Dose rate Dpa/day Ar4066016.50150 2.75 10002 Kr84120114.309610.185004164 12 II.Intermediate energy irradiation at ATLAS- Argonne Post-irradiation characterization: Hot cells at Irradiated material Lab Tensile testing - Fracture toughness - Fatigue TEM / TEM The LECO machines for measuring oxygen, nitrogen and hydrogen contents of the irradiated samples. 2.Heavy ion irradiation: Slide 13 References 13 Rodchenkov, B.S., M.V. Evseev, Yu.S. Strebkov, L.P. Sinelnikov, and V.V. Shushlebin. Properties of Unirradiated and Irradiated Ti6Al4V Alloy for ITER Flexible Connectors. Journal of Nuclear Materials 417, no. 13 (October 2011) Thtinen, S., P. Moilanen, B. N. Singh, and D. J. Edwards. Tensile and Fracture Toughness Properties of Unirradiated and Neutron Irradiated Titanium Alloys. Journal of Nuclear Materials 307 (2002): 416420. Hegeds, Ferenc, Roland Brtsch, Brian Oliver, and Pierre Marmy. Fracture Toughness and Tensile Properties of the Titanium Alloys Ti6A14V and Ti5A12. 5Sn Before and After Proton and Neutron Irradiations at 150 C. Centre de recherches en physique des plasmas (CRPP), Ecole polytechnique fdrale, 2004.